**http://wrap.warwick.ac.uk/ **

**Original citation: **

### Mudd, James J., Lee, Tien-Lin, Muñoz-Sanjosé, V., Zúñiga-Pérez, J., Payne, D. J.,

### Egdell, R. G. and McConville, C. F. (Chris F.). (2014) Valence-band orbital character of

### CdO : a synchrotron-radiation photoelectron spectroscopy and density functional theory

### study. Physical Review B (Condensed Matter and Materials Physics), Volume 89

### (Number 16). Article number 165305

**Permanent WRAP url: **

### http://wrap.warwick.ac.uk/62980

**Copyright and reuse: **

### The Warwick Research Archive Portal (WRAP) makes this work of researchers of the

### University of Warwick available open access under the following conditions.

### This article is made available under the Creative Commons Attribution- 3.0 Unported

### (CC BY 3.0) license and may be reused according to the conditions of the license. For

### more details see

### http://creativecommons.org/licenses/by/3.0/

**A note on versions: **

### The version presented in WRAP is the published version, or, version of record, and may

### be cited as it appears here.

**Valence-band orbital character of CdO: A synchrotron-radiation photoelectron spectroscopy and**

**density functional theory study**

J. J. Mudd,1,*_{Tien-Lin Lee,}2_{V. Mu˜noz-Sanjos´e,}3_{J. Z´u˜niga-P´erez,}4_{D. J. Payne,}5_{R. G. Egdell,}6_{and C. F. McConville}1,*†*
1_{Department of Physics, University of Warwick, Coventry, CV4 7AL, United Kingdom}

2* _{Diamond Light Source Ltd., Harwell Science and Innovation Campus, Didcot, OX11 0DE, United Kingdom}*
3

*4*

_{Departamento de Fisica Aplicada y Electromagnetismo, Universitat de Val´encia, C/Dr. Moliner 50, 46100 Burjassot, Spain}

_{Centre de Recherche sur lH´et´ero-Epitaxie et ses Applications, Centre National de la Recherche Scientifique, Parc de Sophia Antipolis,}*Rue Bernard Gr´egory, 06560 Valbonne, France*

5_{Department of Materials, Imperial College London, London, SW7 2AZ, United Kingdom}

6_{Inorganic Chemistry Laboratory, Department of Chemistry, University of Oxford, South Parks Road, Oxford OX1 3QR, United Kingdom}

(Received 4 February 2014; revised manuscript received 19 March 2014; published 11 April 2014)
*N*-type CdO is a transparent conducting oxide (TCO) which has promise in a number of areas including
solar cell applications. In order to realize this potential a detailed knowledge of the electronic structure of the
material is essential. In particular, standard density functional theory (DFT) methods struggle to accurately
predict fundamental material properties such as the band gap. This is largely due to the underestimation of the
Cd 4dbinding energy, which results in a strong hybridization with the valence-band (VB) states. In order to test
theoretical approaches, comparisons to experiment need to be made. Here, synchrotron-radiation photoelectron
spectroscopy (SR-PES) measurements are presented, and comparison with three theoretical approaches are made.
In particular the position of the Cd 4dstate is measured with hard x-ray PES, and the orbital character of the
VB is probed by photon energy dependent measurements. It is found that LDA+U using a theoretical U value
of 2.34 eV is very successful in predicting the position of the Cd 4dstate. The VB photon energy dependence
reveals the O 2pphotoionization cross section is underestimated at higher photon energies, and that an orbital
contribution from Cd 5pis underestimated by all the DFT approaches.

DOI:10.1103/PhysRevB.89.165305 PACS number(s): 68.47.Gh,71.15.Mb,79.60.Bm

**I. INTRODUCTION**

CdO is a rocksalt metal oxide which is amenable to*n*-type
doping resulting in high conductivity and optical transparency.
It shows promise for device applications due to its ability to
achieve high*n*-type carrier concentrations (∼1021 _{cm}−3_{) and}
high electron mobilities (220 cm2V−1s−1) [1–3]. It is also a
promising candidate to alloy with ZnO to form Cd*x*Zn1−*x*O,

potentially achieving devices operating across the visible
spectrum [4,5]. However, in order to exploit these potential
applications a detailed knowledge of the electronic structure
of both CdO and ZnO is required [6,7]. In particular, predicting
the band gap of these materials is crucial for most applications.
However, many current theoretical approaches predict CdO to
be a semimetal [8]. This is a result of the underestimation
of the binding energy of the Cd 4*d* states, which results
in strong*p-d* hybridization in the valence band (VB) and a
reduction of the band gap. There have been several theoretical
attempts to correct this problem including the use of hybrid
functionals [9,10] and GW quasiparticle calculations [11,12].
These approaches have had some success in predicting the
location of the shallow Cd 4*d*states and the band gap; however,
they are also computationally more complex and therefore less
widely applied. An alternative approach is LDA+U [13–15],
where an on-site, orbital dependent Coulomb term is added to
the local density approximation (LDA) potential. This allows
the position of the Cd 4*d* states to be corrected and should
therefore improve the associated theoretical predictions.

*_{j.j.mudd@warwick.ac.uk}

*†*_{c.f.mcconville@warwick.ac.uk}

In order to assess the merits of these theoretical
ap-proaches, comparisons with experimental data need to be
made. Photoemission is an ideal technique for this as it
essentially allows the VB density of states (DOS) to be
observed. To the best of our knowledge there have been
two previous publications comparing theoretical predictions
to experimental photoemission data for CdO, King*et al.*[16]
and Dou*et al.*[17]. This work significantly extends both of
these comparisons, by both the use of additional theoretical
approaches and synchrotron-radiation techniques.

Synchrotron-radiation excited photoelectron spectroscopy
(SR-PES) has been used to obtain both hard x-ray
photoemis-sion (HAXPES) data of the CdO VB and Cd 4*d* regions for
comparison to density functional theory (DFT), and a series of
CdO VB spectra over a range of photon energies to allow the
VB orbital character to be investigated in more detail. With its
higher incident photon energy, HAXPES is a preferred
tech-nique when comparing to theoretical calculations as it is more
bulk sensitive than traditional photoemission [18], allowing
for better comparison with the theoretical bulk calculations.
It is also of benefit that photoionization cross sections are
smoothly varying at high photon energies, allowing trends to
be more easily observed. Theoretically three DFT functionals
were chosen (LDA, PBE-GGA, and LDA+U), due to their
widespread availability and relative computational simplicity.

**II. EXPERIMENTAL DETAILS**

Epitaxial CdO(100) single crystal thin films were grown on

J. J. MUDD*et al.* PHYSICAL REVIEW B**89, 165305 (2014)**

elsewhere [21]. The sample was prepared in ultra-high vacuum (UHV) by annealing at 550◦C for 45 min, an approach which has previously been shown to be very effective [16]. Prior to the PES measurements the surface order was confirmed by LEED, which showed a sharp (1×1) diffraction pattern indicating high surface quality. Additionally, no contamination was observed during the PES measurements.

Photoemission spectra were obtained at the I09 beamline of
Diamond Light Source, UK. The I09 beamline offers photon
energies from 100 eV to 18 keV, achieved using two canted
undulators, providing both soft and hard x rays focused to
the same point on the sample. Hard x rays (*hν*2500 eV)
were monochromated using a cooled Si(111) double crystal
monochromator. To maintain sufficient energy resolution at the
two highest photon energies an additional Si channel-cut high
resolution monochromator, Si(444) for *hν*=7935 eV and
Si(004) for*hν*=6054 eV, was used. Soft x rays (*hν* =600 eV)

FIG. 1. (Color online) (a) Plan view of the experimental
geome-try used. The photon beam is perpendicular to the analyzer lens axis
and the sample is placed at grazing incidence to the photon beam. The
electric polarization vector is coincident with the analyzer lens axis.
The±30◦angular acceptance of the electron analyzer is illustrated by
the shaded blue triangle. (b) The one-electron photoionization cross
sections and (inset)*β*dipole asymmetry parameters for the orbitals
constituting the CdO valence band. Shown for photon energies 0.1
to 10 keV. Note the logarithmic scale. Data from Trzhaskovskaya
*et al.*[19,20].

were monochromated using a plane grating monochromator
(300 lines*/*mm). The endstation is equipped with a VG Scienta
EW4000 electron analyzer with±30◦angular acceptance. In
the experimental geometry at I09 shown in Fig.1(a), the photon
beam is perpendicular to the electron emission direction. The
photon beam is polarized in the plane of the orbit (horizontally)
resulting in the electric vector being aligned with the electron
emission direction. The sample was placed in a grazing
incidence geometry (∼5◦), with the surface normal in the plane
defined by the photon beam and electron emission direction
(*p*-polarized), thereby significantly enhancing the count rate.
The experiments were performed at room temperature. The
total experimental energy resolution is*<*0*.*6 eV, for all photon
energies. All experimental data are shown with energy scales
referenced to the valence-band maximum (VBM) to allow for
comparison to the theoretical calculations.

**III. COMPUTATIONAL DETAILS**
**A. Density functional theory**

DFT calculations were performed using the full
poten-tial linearized augmented plane wave (FP-LAPW) method
with local orbitals [22], as implemented in the ELK open
source code [23]. Calculations were performed on CdO
in the rocksalt structure. Three different DFT functionals
were applied; Perdew-Zunger local density approximation
(LDA) [24], Perdew-Burke-Ernzerhof generalized gradient
approximation (PBE-GGA) [25], and the LDA+U approach
within the fully localized limit (FLL) [13–15]. The difficulty in
applying this method is choosing a suitable value of U. Here
a theoretically calculated value of *U*=2*.*34 eV suggested
by Janotti *et al.* [26] is used, applied to the Cd 4*d* states.
Structural optimization was conducted with each functional by
performing calculations over a range of unit cell volumes, and
fitting the energy-volume curve with the Murnaghan equation
of state [27]. From this the equilibrium lattice parameter
was obtained, and this was used when calculating the band
structures and partial density of states (PDOS). Convergence
tests with respect to the plane wave cutoff and*k*-point mesh
indicate the results are numerically converged to∼5 meV. The
wave functions inside the muffin tins were expanded up to

*l*max=8 and the plane waves were expanded with a cutoff
of*R*MT

min×*K*max=8*.*5, where*R*minMTis the smallest muffin tin
radius and*K*_{max}= |**G**+**k**|the maximum value of the wave
vector. The muffin-tin radii were chosen as*R*MT_{Cd} =1*.*35 ˚A
and*R*MT

O =0*.*94 ˚A. A*k*mesh of 8×8×8 was found to be
sufficient for all calculations.

**B. Experimental comparison**

DFT has been used to calculate the orbitally resolved
PDOS. To allow comparison with experimental data the PDOS
was multiplied by the one-electron photoionization cross
sections, including an asymmetry correction. To obtain these
one-electron photoionization cross sections, the tabulated
val-ues of the subshell photoionization cross sections, calculated
by Trzhaskovskaya*et al.*[19,20], were summed and divided
by the orbital occupancy of a free atom. As the Cd 5*p*shell is
unoccupied in a Cd atom, the cross section was estimated by
applying the In 5*p/*In 5*s*ratio to the Cd 5*s*cross section. The

Cd 5*p*dipole asymmetry parameter was assumed to be equal to
the In 5*p*dipole asymmetry parameter, a valid approach as the
dipole asymmetry changes only weakly with atomic number.
The resulting one-electron photoionization cross sections and

*β*dipole asymmetry parameters are shown in Fig.1(b).
The differential cross section including the dipolar and
nondipolar asymmetry parameters, for linearly polarized light,
is given by [30]

*dσi*

*d* =

*σi*

4*π*[1+*βP* 2(cos*θ*)

dipolar

+(*δ*+*γ* cos2*θ*) sin*θ* cos*φ*

nondipolar

]*,*

(1)
where*P*2is the Legendre polynomial,*σi*is the photoionization

cross section, *β* is the dipole asymmetry parameter, and *γ*

and *δ* are nondipolar asymmetry parameters. The angle *θ*

is defined between the polarization vector and the electron
emission direction, and *φ* is defined as the angle between
the photon propagation direction and the plane defined by
both the electron emission direction and polarization vector,
which in the experimental geometry used is always zero. As
the nondipolar term displays odd parity, integrating over a
symmetric*θ*range will result in no contribution from this term,
and therefore no dependence on the nondipolar asymmetry
parameters. Considering the±30◦angular acceptance of the
electron analyzer and performing the integration of Eq. (1),
the total cross section can be written as

*σ _{i}*total=

*σi*

96*π*[8*π*+*β*(9
√

3+2*π*)]*.* (2)

This expression is used to calculate the total cross section to be applied to each orbital when weighting the PDOS. The photoionization cross section weighted PDOS were then summed and convolved with a 0.7 eV FWHM Gaussian to account for lifetime and phonon broadening, and the finite experimental resolution.

**IV. RESULTS AND DISCUSSION**
**A. Computational results**

The key numerical results are shown in Table I, which also includes values from recently published hybrid functional (HSE 06) [9], and GW quasiparticle calculations [11]. The calculated lattice parameters agree well with experiment and

TABLE I. Key numerical results from experiment and DFT. The
values shown are lattice parameter*a*and direct (Edir

*G*) and indirect
band gap (Eind

*G* ) (negative values indicate semimetallic). The
valence-band width (VB); location of the Cd 4dstates with respect to the
VBM. All energies are in eV.

*a*( ˚A) *E*dir

*G* *E*

ind

*G* VB 4dstates
Expt. 4.695 [21] 2.18 [28] 0.9 [29] 4.8 −8.70

LDA 4.639 1.12 −0.45 4.72 −6.76

PBE 4.775 0.68 −0.51 3.98 −6.58

LDA+U 4.619 1.34 0.21 4.18 −8.60

HSE 06a _{4.720} _{2.18} _{0.89} _{4.45} _{−}_{7.4}

GWb _{4.650} _{2.88} _{1.68} _{}_{4.75} _{}_{−}_{9}

a_{Hybrid functional calculation, Burbano}_{et al.}_{[}_{9}_{].}
b_{GW quasiparticle calculation, Dixit}_{et al.}_{[}_{11}_{].}

previous theoretical calculations [4,9,11,21]. The calculated
DFT band structures are shown in Fig. 2, where clear
differences between the functionals are visible. Both LDA and
PBE predict CdO to be a semimetal, i.e., the conduction band
minimum is below the VBM. This is clearly not consistent
with experimental evidence, with the most recent optical
measurements placing the direct band gap at 2.18 eV at
room temperature [28] and XANES reporting an indirect gap
of ∼0*.*9 eV [29]. PBE predicts the location of the Cd 4*d*

states to be very similar to LDA but with a slightly narrower
overall width. LDA + U shifts the Cd 4*d* states down by

∼2 eV. This opens a direct band gap of 1.34 eV. Although semiconducting behavior with a nonvanishing indirect gap is now predicted, both the direct and indirect gaps are still too small when compared to experiment. It is worth noting that more sophisticated computational methods such as hybrid functionals [9] can potentially predict the band gap much more accurately.

The partial density of states (PDOS) for each of the
functionals is shown in Figs. 3(a)–3(c). It is of note that,
for all the functionals, the VB DOS is dominated by O 2*p*

character, and the shape of this feature is very similar. PBE
predicts a narrower VB than either LDA or LDA+U. The
most significant difference is in the orbital character of peak
I. LDA predicts this peak to have significant Cd 4*d*character
resulting from the underestimation of the Cd 4*d*states binding
energy. PBE shows the Cd 4*d* character of this peak to be
much reduced giving roughly similar importance to Cd 4*d*

and Cd 5*s*. For LDA + U the Cd 4*d* character of peak I
is further reduced due to the Cd 4*d* states being shifted to
lower energy reducing hybridization. This results in Cd 5*s*

contributing more to the DOS in peak I than Cd 4*d*. The Cd
5*p* and O 2*s* components are also shown. These are often
excluded due to their small contributions. However, at higher
photon energies their importance to VB-PES increases as their
photoionization cross section drops off much less rapidly than
O 2*p*as shown in Figs.1and5.

**B. Experimental comparison**

A comparison between the three DFT functionals and
experimental valence-band photoemission spectroscopy
(VB-PES) measurements taken with a photon energy of 6054 eV is
shown in Figs.3(d)–3(i). The higher photon energy compared
to earlier studies [16,17] decreases the surface sensitivity,
which is beneficial in the case of CdO as it is known to
exhibit surface electron accumulation [31,32], which is not
representative of the bulk electronic properties. A Shirley
background [33] has been subtracted across the whole region.
The PDOS shown in Figs.3(a)–3(c) have been weighted using
the photoionization cross sections and asymmetry corrections
appropriate for a photon energy of 6054 eV and then summed,
as shown by the shaded gray region. The sum of weighted
PDOS was then convolved with a 0.7 eV FWHM Gaussian,
resulting in the red line. The experimental spectra and
convolved DFT are normalized to peak II of the VB, and
the same normalization was applied to both the VB and Cd 4*d*

J. J. MUDD*et al.* PHYSICAL REVIEW B**89, 165305 (2014)**

-10 -8 -6 -4 -2 0 2 4 6 8 10

Ener

gy (eV)

Γ X W K Γ L W

LDA

Γ X W K Γ L W Γ X W K Γ L W

PBE LDA+U

(a) (b) (c)

-10 -8 -6 -4 -2 0 2 4 6 8 10

FIG. 2. (Color online) DFT band structures for (a) LDA, (b) PBE, and (c) LDA+U. Blue and red lines denote conduction and valence bands, respectively, the blue shaded region shows the band gap. Note the overlap of the conduction and valence bands predicted by LDA and PBE indicating a semimetallic system. Also note the shift in Cd 4dstates at around−8 eV produced by LDA+U.

Normalized Intensity (arb. units)

25

20

15

10

5

0

-11 -10 -9 -8 -7 -6

Energy (eV)

2.5

2.0

1.5

1.0

0.5

0.0 -5 -4 -3 -2 -1 0 1

2.5

2.0

1.5

1.0

0.5

0.0 2.5

2.0

1.5

1.0

0.5

0.0 3.0

Normalized Intensity (arb. units)

25

20

15

10

5

0 25

20

15

10

5

0

-1

-1

Density of states (states Ha

u.c.

)

Energy (eV) -4 -3 -2 -1 0

Cd 5*s*

Cd 5*p*

Cd 4*d*

O 2*s*

O 2*p*

(a) LDA

(b)

(c) LDA+U 50

40

30

20

10

0 50

40

30

20

10

0 50

40

30

20

10

0

PBE

DFT PDOS Cd 4*d* region VB Region

(d) LDA

(e) PBE

(f) LDA+U

(g)

(h)

(i)

VB-PES DFT DOS Conv. DFT

I II

I

II

FIG. 3. (Color online) (a)–(c) DFT partial density of states calculated using (a) LDA, (b) PBE, and (c) LDA+U. The peak labels I and
II in (a), derived from experimental data, refer to the energy ranges−4.5 to−3 eV and−3 to 0 eV, respectively. (d)–(i) Cd 4dand VB PES
spectra compared to DFT, (d) and (g) LDA, (e) and (h) PBE, and (f) and (i) LDA+U. The DFT PDOS are weighted by the photoionization
cross sections and summed, shown by the gray shaded areas. The weighted PDOS after convolution with a 0.7 eV FWHM Gaussian are shown
by the red line. The experimental data (blue circles) shown is taken with*hν*=6054 eV, and a Shirley background has been subtracted. All
energy scales are referenced to the VBM. The experimental spectra and convolved DFT are normalized to the maximum of VB peak II, and
the same normalization has been applied to both the VB and Cd 4dregions; note the different intensity scales.

agreement with other photoemission measurements [16,17].
Very significant differences between these functionals can
be observed, as discussed previously. LDA and PBE place
the Cd 4*d* states at approximately the same energy, and
this is approximately 2 eV shallower than measured by
experiment. LDA+U corrects for this disagreement extremely
successfully, placing the Cd 4*d*states in very good agreement
with the experimental data. This can also be compared to
recent hybrid functional calculations placing the Cd 4*d*states
at−7*.*4 eV [9] and to a recent GW quasiparticle calculation
which places the Cd 4*d*states at∼−9 eV [11]. It is interesting
to note, however, that the shape of the Cd 4*d* states is better
reproduced by LDA which shows two resolvable peaks as seen
in the experiment. Due to the decreased interaction between
the Cd 4*d* states and the VB predicted by LDA +U, and
to a lesser extent PBE, the DOS within the Cd 4*d* states is
increased. This results in these functionals overestimating the
spectral weight of these states relative to the VB.

The VB region shown in panels (g)–(i) of Fig.3 exhibits
a two peak structure which is correctly reproduced by all the
DFT functionals. However, it can be seen that all the DFT
functionals underestimate the VB width, particularly PBE.
This is consistent with previous results [16]. This also means
that VB peak I is placed too shallow by around 0.5 eV when
compared to the experimental data. The shape of peak II is
best reproduced by LDA, which predicts a slightly wider peak
than PBE or LDA+U. This is partly due to LDA assigning
increased Cd 4*d* character to VB peak II. This is, however,
offset by the fact that LDA also places the Cd 4*d* states
much too shallow resulting in this effect. The additional Cd
4*d* character is also responsible for LDA giving VB peak I
more spectral weight than observed in the experimental data.
The relative intensities of peaks I and II in the VB region
is best reproduced by LDA +U, which still overestimates
peak I intensity.

Figure 4(a) shows VB-PES taken with photon energies ranging from 600 eV to 7935 eV. This approach allows the orbital character of VB to be identified by exploiting the change in photoionization cross sections. The spectra have been normalized to the maximum of VB peak II, following a Shirley background subtraction, to allow relative changes

to be observed. The key changes in the VB shape observed experimentally are indicated by the two arrows labeled 1 and 2 in Fig. 4(a). Arrow 1 shows that peak I of the VB increases strongly with photon energy relative to peak II. Arrow 2 indicates the region in the center of the VB which also increases relative to peak II, and this appears, like a broadening of peak II, with photon energy. Figures4(b)–4(d) show the summed DFT PDOS after weighting with different photoionization cross sections as appropriate for each photon energy, and a convolution with a 0.7 eV FWHM Gaussian (as before) to allow direct comparison to the experimental data.

It can be seen qualitatively that the DFT simulations
reproduce the trend of peak I increasing in relative intensity
with photon energy, but none of the functionals reproduce
this behavior quantitatively. The experimental data at the
lowest photon energy shows peak I weaker than peak II. DFT
doesn’t predict any orbitals with lower PDOS in peak I than
peak II, indicating the orbital character of the VB predicted
by DFT cannot be correct. This result is independent of
the photoionization cross sections applied. However, it can
be seen that reducing the Cd 4*d* contribution to peak I,
which is achieved by LDA+U, does significantly improve
the experimental agreement. In the experimental data the
relative intensity of peak I increases consistently towards
the highest photon energy, whereas the simulations predict
an initially rapid increase which slows toward the highest
photon energy. To address this photon energy dependence,
it seems likely that the photoionization cross sections may
exhibit a more complex energy dependence than encapsulated
by the one-electron cross sections applied here. The rate of
decrease of the O 2*p*one-electron cross section with photon
energy appears to be overestimated here, as this would result
in the more rapid relative increase in peak I intensity with
photon energy, as illustrated by the DFT models. Similar
conclusions regarding the O 2*p*photoionization cross sections
being underestimated at higher photon energies were reached
in the case of*β*-PbO2[34,35] and In2O3[36], where alternative
photoionization cross sections calculated by Scofield [37] and
by Yeh and Lindau [38] were applied.

A possible explanation is that the very low O 2*p* cross
section at higher photon energies is susceptible to enhancement

3.0

2.5

2.0

1.5

1.0

0.5

0.0

Energy (eV)

Normalized intensity (arb. units)

-5 -4 -3 -2 -1 0

Photon Energy 7935 eV 6054 eV 4500 eV 2500 eV 600 eV

-5 -4 -3 -2 -1 0 -5 -4 -3 -2 -1 0 -5 -4 -3 -2 -1 0 (a) Experimental (b) LDA (c) PBE (d) LDA+U

II I

1

2

3.0

2.5

2.0

1.5

1.0

0.5

0.0

J. J. MUDD*et al.* PHYSICAL REVIEW B**89, 165305 (2014)**

FIG. 5. (Color online) The VB region calculated with LDA+U showing the PDOS weighted by photoionization cross sections for photon energies (a) 600 eV and (b) 7935 eV. This allows the effects of the photon energy on the orbital components to be observed.

by interchannel coupling with the much stronger O 2*s* or O
1*s* ionizations. Drube *et al.* [39] have recently shown that
interchannel coupling of this sort may be significant well above
threshold. In support of this idea we note that the agreement
between theory and experiment does significantly improve
with increasing photon energy. It is also interesting to note
that the intensity ratio of peak I to II is quite well reproduced
by all the DFT functionals at the highest photon energy. At
this photon energy the VB-PES is dominated by Cd character,
whereas at the lowest photon energy Cd and O contribute
approximately equally, as shown in Fig.5. This might suggest
that the photoionization cross sections are most accurate within
an element and may contribute a larger error when comparing
orbital character of two or more elements.

The increasing intensity in the center of the VB with
photon energy, shown by arrow 2 at approximately−2*.*7 eV
in Fig.4(a), is most probably a result of Cd 5*p*character in
the center of the VB. The Cd 5*p*photoionization cross section
decreases much less rapidly than O 2*p* with photon energy,
so at higher photon energies its contribution becomes much
more significant (see Fig.5). While all the DFT functionals
predict some Cd 5*p*character, it seems likely this contribution
is underestimated, as the experimental data shows a much
more significant change. Alternatively, the photoionization
cross section for Cd 5*p* could be underestimated at higher
photon energies. While this is possible due to the extrapolation
required to obtain it, it would not be consistent with the trend
in peak I which would then show a stronger photon energy
dependence if this cross section was increased.

**V. CONCLUSIONS**

The VB electronic structure of CdO has been investigated with SR-PES, and comparisons to three DFT functionals have

been made. The location of the Cd 4*d* states which have
a significant effect on the theoretical predictions was not
reproduced by either LDA or PBE-GGA. However, LDA+U
applied using a theoretically calculated U value of 2.34 eV
was very successful in predicting the location of these states.
Experimentally, the VB shows a two peak structure which is
correctly reproduced by all the DFT functionals. However, the
VB width is underestimated in each case, and the application
of LDA + U does not improve this. The photon energy
dependence of the VB-PES was measured and compared to the
theoretical predictions. All the DFT functionals qualitatively
reproduced the observed behavior, with LDA+U again being
the most accurate. The data obtained with the lowest photon
energy indicated the orbital character of the VB was not
completely reproduced by the DFT calculations. Additionally
the center of the VB shows a photon energy dependence which
wasn’t adequately replicated by any of the DFT functionals.
This was assigned to Cd 5*p*character and suggests it is
under-estimated by the DFT approaches. The trends observed with
photon energy indicate that the O 2*p* photoionization cross
section decreases too rapidly with increasing photon energy
when compared with the experimental data. This trend is in
agreement with observations made in previous studies [34–36].
The change in VB shape with photon energy highlights
the potential for this kind of approach in understanding
orbital character present in the VB, and by varying the
polarization even more detailed information can be obtained
by allowing certain orbital character to be suppressed. In
order to exploit this information further, improvements in
the photoionization cross sections at the high photon energies
relevant for HAXPES or one-step photoemission calculations
will be required. All the DFT functionals applied here
significantly underestimate the CdO band gap despite their
successes in predicting the VB shape and Cd 4*d*position. This
clearly illustrates the need for more sophisticated theoretical
approaches such as hybrid functionals and GW quasiparticle
methods, when investigating these materials. It is anticipated
that these experimental results will be of use when assessing
the successes of these approaches.

**ACKNOWLEDGMENTS**

We are grateful to P. K. Thakur (Diamond Light Source, UK) for assistance with SR-PES measurements, and ac-knowledge the EPSRC for the award of a DTA studentship (J.J.M.). The work undertaken at the Universitat de Val´encia was supported by the Spanish Government under Project No. TEC2011-28076-C02-02, and Generalitat Valenciana under the projects Prometeo/2011-035 and ISIC/2012/008, Institute of Nanotechnologies for Clean Energies. The Science City Research Alliance (SCRA) and the European Research and Development Fund (ERDF) are acknowledged for capital equipment investment at Warwick. Diamond Light Source are thanked for awarding beamtime under the proposal SI 8441.

[1] K. M. Yu, M. A. Mayer, D. T. Speaks, H. He, R. Zhao, L. Hsu,
S. S. Mao, E. E. Haller, and W. Walukiewicz,J. Appl. Phys.**111**,

123505(2012).

[2] T. J. Coutts, D. L. Young, X. Li, W. P. Mulligan,
and X. Wu, J. Vac. Sci. Technol. A **18**, 2646

(2000).

[3] R. Chandiramouli and B. Jeyaprakash,Solid State Sci.**16**,102

(2013).

[4] R. Miloua, F. Miloua, A. Arbaoui, Z. Kebbab, and
N. Benramdane,Solid State Commun.**144**,5(2007).

[5] A. Schleife, C. R¨odl, J. Furthm¨uller, and F. Bechstedt,New J.
Phys.**13**,085012(2011).

[6] P. D. C. King and T. D. Veal,J. Phys. Condens. Matter **23**,

334214(2011).

[7] L. Y. Lim, S. Lany, Y. J. Chang, E. Rotenberg, A. Zunger, and
M. F. Toney,Phys. Rev. B**86**,235113(2012).

[8] A. Schleife, F. Fuchs, J. Furthm¨uller, and F. Bechstedt,Phys.
Rev. B**73**,245212(2006).

[9] M. Burbano, D. O. Scanlon, and G. W. Watson,J. Am. Chem.
Soc.**133**,15065(2011).

[10] F. Labat, P. Baranek, C. Domain, C. Minot, and C. Adamo,J.
Chem. Phys.**126**,154703(2007).

[11] H. Dixit, D. Lamoen, and B. Partoens,J. Phys. Condens. Matter

**25**,035501(2013).

[12] A. Schleife, F. Fuchs, C. R¨odl, J. Furthm¨uller, and F. Bechstedt,

Phys. Status Solidi**246**,2150(2009).

[13] V. I. Anisimov, J. Zaanen, and O. K. Andersen,Phys. Rev. B**44**,

943(1991).

[14] A. I. Liechtenstein, V. I. Anisimov, and J. Zaanen,Phys. Rev. B

**52**,R5467(1995).

[15] V. I. Anisimov, F. Aryasetiawan, and A. I. Lichtenstein,J. Phys.
Condens. Matter**9**,767(1997).

[16] P. D. C. King, T. D. Veal, A. Schleife, J. Z´u˜niga-P´erez, B. Martel,
P. H. Jefferson, F. Fuchs, V. Mu˜noz-Sanjos´e, F. Bechstedt, and
C. F. McConville,Phys. Rev. B**79**,205205(2009).

[17] Y. Dou, R. G. Egdell, D. S. L. Law, N. M. Harrison, and B. G.
Searle,J. Phys. Condens. Matter**10**,8447(1998).

[18] J. J. Mudd, T. L. Lee, V. Mu˜noz-Sanjos´e, J. Z´u˜niga-P´erez,
D. Hesp, J. M. Kahk, D. J. Payne, R. G. Egdell, and C. F.
McConville,Phys. Rev. B**89**,035203(2014).

[19] M. Trzhaskovskaya, V. Nefedov, and V. Yarzhemsky,At. Data
Nucl. Data Tables**77**,97(2001).

[20] M. Trzhaskovskaya, V. Nikulin, V. Nefedov, and V. Yarzhemsky,

At. Data Nucl. Data Tables**92**,245(2006).

[21] J. Zu˜niga P´erez, C. Munuera, C. Ocal, and V. Mu˜noz-Sanjos´e,

J. Cryst. Growth**271**,223(2004).

[22] D. Singh and L. Nordstr¨om,*Planewaves, Pseudopotentials, and*
*the LAPW method, 2nd ed. (Springer, New York, 2005).*

[23] “Elk FP-LAPW DFT Code,”http://elk.sourceforge.net/.
[24] J. P. Perdew and A. Zunger,Phys. Rev. B**23**,5048(1981).
[25] J. P. Perdew, K. Burke, and M. Ernzerhof,Phys. Rev. Lett.**77**,

3865(1996).

[26] A. Janotti, D. Segev, and C. G. Van de Walle,Phys. Rev. B**74**,

045202(2006).

[27] F. D. Murnaghan, Proc. Natl. Acad. Sci. USA **30**, 244

(1944).

[28] S. K. Vasheghani Farahani, V. Munoz-Sanjose, J. Zuniga-Perez,
C. F. McConville, and T. D. Veal,Appl. Phys. Lett.**102**,022102

(2013).

[29] I. N. Demchenko, J. D. Denlinger, M. Chernyshova, K. M. Yu,
D. T. Speaks, P. Olalde-Velasco, O. Hemmers, W. Walukiewicz,
A. Derkachova, and K. Lawniczak-Jablonska,Phys. Rev. B**82**,

075107(2010).

[30] J. W. Cooper,Phys. Rev. A**47**,1841(1993).

[31] P. D. C. King, T. D. Veal, C. F. McConville, J. Z´u˜niga-P´erez,
V. Mu˜noz-Sanjos´e, M. Hopkinson, E. D. L. Rienks, M. F. Jensen,
and P. Hofmann,Phys. Rev. Lett.**104**,256803(2010).
[32] L. F. J. Piper, L. Colakerol, P. D. C. King, A. Schleife,

J. Z´u˜niga-P´erez, P. A. Glans, T. Learmonth, A. Federov,
T. D. Veal, F. Fuchs, V. Mu˜noz-Sanjos´e, F. Bechstedt, C. F.
McConville, and K. E. Smith,Phys. Rev. B**78**,165127(2008).
[33] D. A. Shirley,Phys. Rev. B**5**,4709(1972).

[34] D. J. Payne, R. G. Egdell, G. Paolicelli, F. Offi, G. Panaccione,
P. Lacovig, G. Monaco, G. Vanko, A. Walsh, G. W. Watson,
J. Guo, G. Beamson, P.-A. Glans, T. Learmonth, and K. E.
Smith,Phys. Rev. B**75**,153102(2007).

[35] D. J. Payne, G. Paolicelli, F. Offi, G. Panaccione, P. Lacovig,
G. Beamson, A. Fondacaro, G. Monaco, G. Vanko, and
R. G. Egdell, J. Electron Spectrosc. Relat. Phenom. **169**, 26

(2009).

[36] C. K¨orber, V. Krishnakumar, A. Klein, G. Panaccione, P. Torelli,
A. Walsh, J. L. F. Da Silva, S.-H. Wei, R. G. Egdell, and D. J.
Payne,Phys. Rev. B**81**,165207(2010).

[37] J. Scofield, Lawrence Livermore Lab. Report No. UCRL-51326, 1973 (unpublished).

[38] J. Yeh and I. Lindau, At. Data Nucl. Data Tables **32**, 1

(1985).